# 1 8.511 Theory of Solids I

```1
8.511 Theory of Solids I
Problem Set 4
Due October 12, 2004
1. The electronic structure of La2 CuO4 is believed to be well described by a two dimensional
square planar model of copper with oxygen mid-way between the nearest neighbor copper
atoms. (See top and bottom layers in Fig. 1.)
Due to the distortion of the oxygen octahedra, the highest energy d orbital on the copper
site is described by a single dx2 −y2 orbital with energy Ed . We use the approximation of
retaining the degenerate px , py with orbitals at energy Ep on the oxygen sites.
(a) Retain the only tight binding matrix elements between the copper and nearest neighbor
oxygen orbitals (you may ignore the overlap matrix element due to non-orthogonality),
and calculate the tight binding band structure.
(b) Assume that La is in the 3+ ionic state and the oxygen oﬀ the plane is purely 2–. With
the further assumption that the 4s level on copper is unoccupied, show that there is
2
one hole per unit cell in the d, p, orbitals that we kept. Locate the Fermi level in your
band structure. Determine the Fermi surface.
(c) Locate the saddle points on the Fermi surface and show that the density of states is
logarithmically divergent at energy near the Fermi energy.
(d) Sketch the Fermi surface when 15% of the La3+ is replaced by Sr2+ . This is called hole
doping. For a determination of the Fermi surface using angular resolved photoemission,
see Yoshida et al., Phys. Rev. B 63, 220501 (2001).
(e) L. Mattheiss [Phys. Rev. Lett. 58, 1028 (1987)] has computed the band structure
using a modiﬁed APW method. He claims that the band structure is well ﬁtted by a
tight binding model with Ep = Ed and a matrix element of –1.85 eV. Check this claim.
Note that Mattheiss takes into account interlayer coupling which leads
in
� to dispersion
�
the c direction. Consequently we can identify his X and S with our πa ,
πa and Γ and
Z with our (0,0).
```